57 EPITAXIAL FILM GROWTH OF THE CHARGE- . . . 12 531
organic solvents. Substrates are then glued with silver paint
on a heater block that is situated opposite to the target at a
distance of 4.7 cm. A polycrystalline Rb 0.30MoO 3 target is
placed in a pulsed-laser beam. The illuminated area is about
5 mm 2 . The background pressure in the deposition chamber
is 10 6 Torr. During deposition the target rotates and depo-
sition takes place in an oxygen atmosphere. To obtain single-
phase blue-bronze ﬁlms the substrate temperature is kept be-
tween 375 °C and 500 °C and the oxygen pressure between
100 and 175 mTorr. Films were grown with thicknesses
ranging from 1.5 to 1000 nm. Film thicknesses ranging from
300 to 1000 nm were determined by measuring the depth
proﬁle across a cut through the ﬁlm with a Tencor Instru-
ments -step 200 proﬁlometer. Thinner ﬁlms were obtained
by adjusting the deposition time. More details about the ﬁlm
growth have been presented elsewhere.4,5
After deposition, various analysis techniques have been
used for characterization of the blue-bronze ﬁlms such as
AFM, transmission electron microscopy, scanning electron
microscopy, scanning tunneling microscopy STM , optical
microscopy, and x-ray diffraction. In this paper we discuss in
detail the results obtained from AFM and x-ray diffraction.
AFM was done with a Nanoscope III in air at room tempera-
The diffraction experiments on ﬁlms with a thickness
from 300 to 1000 nm were carried out with a four-circle FIG. 1. AFM images of the surface of a blue-bronze ﬁlm on
diffractometer. The Cu K x-ray beam was taken from a SrTiO 3 001 . a Small islands are observed for ﬁlm thicknesses of
standard laboratory source run at 20 mA and 40 kV. Slits 2 nm, whereas in b for a ﬁlm thickness of 300 nm, the surface is
were used to deﬁne the primary beam and the acceptance covered with much larger, uniformly shaped clusters.
angle of the detector. The width of the primary beam in the
scattering plane was 0.10°, and a Ni ﬁlter was used to elimi- ﬁlm-substrate relation and the crystalline quality have been
nate the K contribution in the wavelength spectrum. investigated. The ﬁlm-substrate relation is determined from
The x-ray measurements on two blue-bronze ﬁlms with a the in-plane and out-of-plane orientation of the crystal axes
thickness of 2 nm were performed on the vertical scattering of both the substrate and the adlayer. The crystalline ﬁlm
diffractometer at the BW2 wiggler beamline in HASYLAB quality is inspected with respect to the correlation length, the
DESY Hamburg . The photon energies used for the diffrac- strain, and the texture. Measurements have been performed
tion experiments at the two samples were 8.6 and 9.0 keV, on two samples grown at 375 °C and 410 °C, which gave
respectively. The angle of grazing incidence was kept con- similar results.
stant and equal to 0.5°. All diffraction measurements were The out-of-plane growth direction for blue bronze is
performed in air at room temperature. ¯
(201 only, which means that the layers grow plane-parallel
to the surface. The orientation of the in-plane b axis in the
III. EXPERIMENTAL DATA adlayer has been determined from the intensity distribution
on the 020 in-plane circle. This intensity proﬁle describes
A. Initial stage of growth
all possible directions of the b * axes. In Fig. 2 a , the proﬁle
The initial growth of blue bronze on SrTiO 3 001 has at the 020 circle is shown in which the substrate is oriented
been studied on ﬁlms with a thickness between 1 and 10 nm. such that the principal axes are along 0° and 90°.
The ﬁlm thickness is equivalent to the thickness of a con- The background signal is due to scattering from Vaseline
tinuous ﬁlm with the same amount of material. The data used to mount the sample on the diffractometer. The four
presented here were taken on ﬁlms with an equivalent layer maxima in the 020 intensity proﬁle correspond to orienta-
thickness of 2 nm. A typical AFM image is shown in Fig. tions of the b axes parallel to the principal axes of the sub-
1 a in which 3D island nucleation is clearly visible. The strate.
typical length scale of the dropletlike-shaped islands is 150 To estimate the crystalline quality in the ﬁlm, the width
50 nm. Their height is about 10 nm. The sample in Fig. and the position of several independent reﬂections have been
1 a was grown at 440 °C and the island density is about 30 inspected. In general, the tangent width of the reﬂections
m 2 . We have systematically studied the initial stage of i.e., the width of the reﬂections along a circle in the plane of
growth as a function of growth temperature and deposition the surface is due to a combination of a correlation length
rate. Island growth dominates in all cases. The density of the reduction and a crystalline orientation distribution. A ﬁnite-
islands varies only slightly with deposition temperature or size effect results in a broadening independent of the radial
deposition rate. position. An orientation distribution leads to a broadening
More information about these ultrathin ﬁlms is obtained with a linear dependence on the radial distance. The tangent
by means of synchrotron x-ray diffraction. In particular, the widths of the blue-bronze 0 2n 0 reﬂections with n 1, 2,
12 532 A. J. STEINFORT et al. 57
FIG. 3. The intensity distribution from a 300-nm-thick ﬁlm re-
corded through the main 221 and the 403 reﬂections. In a the
circle parallel to the surface is scanned showing four main in-plane
crystalline orientations. In b the intensity is recorded by rotating
the sample around the b axis.
FIG. 2. X-ray-diffraction measurements from a 2-nm-thick ﬁlm.
a The scattering proﬁle recorded on the in-plane 020 circle 10–50 nm. At coverages equivalent to 15 nm and more,
showing the preferred crystalline orientations. b The width in AFM images show the formation of larger, uniformly shaped
SrTiO 3 rlu of the 0 2n 0 reﬂections along a circle in the plane of clusters. A typical AFM image of a 300-nm-thick ﬁlm is
the surface. From the slope and the offset of the linear ﬁt through shown in Fig. 1 b . This ﬁlm is grown at the same tempera-
the data points the in-plane orientation distribution and the particle ture and deposition rate as the ﬁlm in Fig. 1 a . Clearly, the
size are estimated. density of the clusters is signiﬁcantly less than the island
density at the initial stage of growth. In contrast to ﬁlms at
and 3 are shown in Fig. 2 b as a function of the radial the initial stage of growth, we ﬁnd that both the island den-
distance in reciprocal space. The distances are expressed in sity and grain sizes of the thick ﬁlms are strongly tempera-
SrTiO 3 reciprocal lattice units rlu with h parallel to the ture dependent. Island density varies from 10 m 2 at
blue-bronze b * axis and k in the in-plane direction perpen- 375 °C to 3 m 2 at 440 °C. Grain sizes range from 0.3
dicular to it. The linear ﬁt through the data points is shown as
0.5 m2 at 375 °C to 1 5 m 2 at 440 °C. In general,
a solid line. The slope of this solid line corresponds to the
thick ﬁlms consist of grains that are about 10–100 times
orientation distribution, and from the intersection with the y larger than the islands at the initial growth stage.
axis the island size can be estimated. As can be seen in Fig. Grains in thick ﬁlms have a form that is very different
2 b , the peak broadening is almost entirely due to an orien- from the dropletlike shape. As can be seen in Fig. 1 b , elon-
tation distribution of 1.11°. The intersection of the linear ﬁt gated grains grow in two perpendicular directions. Section
with the y axis corresponds to an island size of 200 nm. As analysis on the height proﬁles shows that the clusters are
the intersection is close to the origin, the relative error is asymmetrically bound by facets along the long side. The
large, but the estimate of 200 nm equals the size of the is- facet planes are well deﬁned and make preferred angles with
lands as deduced from AFM images. Apparently, the islands the substrate. The angles of more than 1000 facets have been
are monocrystalline. measured by the AFM and plotted in a histogram see Fig.
The strain in the ﬁlm has been deduced from the positions 5 b . From this histogram the preferred angles are estimated
of the in-plane 020 reﬂection together with thirteen inde- to be 7°, 14°, 18°, 22°, 30°, 32°, and 39°. Angles larger
pendent reﬂections. Strain shows up as an asymmetric peak than 50° were impossible to measure by AFM because of
proﬁle or in a shift of the peak position. No asymmetry or convolution between the tip and the surface proﬁle.
positional shifts with respect to the bulk reﬂection positions The ﬁlm texture and relative orientations of the islands
have been found up to 0.1%. This implies that the initial have been studied by means of x-ray diffraction. Measure-
islands are fully relaxed. The relaxed, monocrystalline crys- ments are performed on ﬁlms with a thickness ranging from
tal formation on the surface with an orientation distribution 200 to 1000 nm. In general, the in-plane and out-of-plane
of over 1° suggests a very weak ﬁlm-substrate bonding. In texture decreases by increasing the ﬁlm thickness. The out-
spite of this weak bonding, heteroepitaxial ﬁlm growth is of-plane growth direction of the blue-bronze layers remains
observed: the ﬁlms are oriented with the (201 slabs parallel ¯ ¯
mainly (201 . Only a minor part of the ﬁlm is (403 oriented
to the substrate surface and the b axis oriented along the as has been estimated from an out-of-plane -2 x-ray scan.
substrate principal axes. ¯
The in-plane orientation of the (201 clusters has been
investigated from the intensity proﬁles on the surface-
B. Thick Rb 0.30MoO 3 ﬁlms on SrTiO 3 „100… ¯ ¯
parallel circles through the 221 and the 403 reﬂections.
Continuation of the deposition of blue bronze leads to a An example of the scattering proﬁles is shown in Fig. 3 a .
full coverage of the surface at a layer thickness of about The substrate principal axes are oriented along the 0°
57 EPITAXIAL FILM GROWTH OF THE CHARGE- . . . 12 533
and the 90° directions. For clarity, the intensity proﬁles
around the maxima are shown on a larger intensity scale. The
similar shape of the proﬁles shows the azimuthal orientation
distribution of the (201 clusters. The four main intensity
maxima in Fig. 3 a result from clusters that are oriented
with the b axes along the substrate principal axes. The width
of the maxima is 1.3°, slightly more than the width of the
peaks in Fig. 2 a . In general, we ﬁnd that for thick ﬁlms the
in-plane width of the maxima is substantially more than 1°
typically, it varies between 2° and 7°. In addition to the main
orientations along the substrate axes, intermediate orienta-
tions are present that make an angle of 27° and 45° with the
substrate principal axes. The width of these maxima is about
10°. Both the broadening of the peaks and the observation of
additional orientations indicate a reduced in-plane texture for FIG. 4. The lateral intensity proﬁle of a 300-nm-thick blue-
thick ﬁlms. bronze ﬁlm recorded at different heights in reciprocal space. Extra
The out-of-plane orientation shows a similar trend as reﬂections are visible on both sides of the rod through the blue
found for the in-plane orientation, less texture with increas- bronze ¯01 as a result of the facets on the blue-bronze clusters.
ing ﬁlms thickness. All additional out-of-plane orientations, The reﬂections run in a direction 55° with the surface. In a the
however, have the b axes in the plane of the surface. In Fig. reﬂections coincide at the blue bronze 020 at l 0 and in b they
3 b the proﬁles through the main 221 and 403 reﬂections coincide at blue bronze ¯21 at l 0.473.
are shown. The x axes in these plots indicate a rotation
around the b axis. The proﬁles clearly contain several side pal axes of the substrate. The relaxed state of the islands
peaks next to the main reﬂection. We have checked that the indicates a weak ﬁlm-to-substrate bonding. This weak bond-
side peaks do not result from a superperiodicity. The main ing may also be responsible for the in-plane mosaic spread of
reﬂection belongs to a ¯01 -oriented material and the side
2 1.1°. At an average ﬁlm thickness of 10–50 nm, the surface
peaks result from blue bronze with tilted 201 planes. The is fully covered with islands. Between the closed-packed is-
tilt angles equal 7°, 14°, and 18°. In the conventional unit lands, grain boundaries will appear as a result of the discrep-
cell description, most of these orientations do not result in ancy between the unit nets of the substrate surface and the
low-index planes parallel to the surface except for the peak ﬁlm. The grain boundaries will limit the correlation length to
near 18°. Rotation of the ¯01 slabs over 18° around the b
2 the size of the islands. At higher coverages a change in the
axis results in 403 -oriented material, in agreement with the growth appears. Larger, highly uniform, elongated clusters
-2 scans. start to form with dimensions 10–100 times larger than the
With synchrotron x-ray diffraction, it is in principle pos- initial islands. The grain density is considerably smaller than
sible to measure facet angles if the facets are well deﬁned at the initial stage of growth. In both the in-plane and the
and have dimensions of tens of nanometers or larger. Cluster out-of-plane direction the number of preferred orientations
faceting results in the appearance of intensity rods in recip- and the mosaic spread increases.
rocal space parallel to the facet normal9 analogous to the Our observations suggest three distinct stages of growth.
appearance of crystal truncation rods as a result of the pres- In the initial stage, small monocrystalline islands nucleate at
ence of a crystal surface. An example is shown in Fig. 4. the substrate surface. Growth of these islands proceeds until
Three proﬁles are shown, recorded in the surface-parallel full coverage. In the second stage, overgrowth of large clus-
direction along a principal axis at different heights in recip- ters bounded by well-deﬁned facets occurs. Since these clus-
rocal space. The central peak in the proﬁles is the crystal ters cover several uncorrelated initial islands, a decrease in
truncation rod as a consequence of the surface. On both sides the in-plane texture is expected. This decrease is, for in-
of the central peak, minor peaks are visible. These side peaks stance, evident in the observed increase of the in-plane mo-
form a line of intensity that makes an angle of 55° with the saic spread. The third stage of growth is characterized by
surface. The peak broadening due to the orientation distribu- ¯
growth of 201 slabs over the facets.
tion prohibits the observation of facet angles smaller than The model for the second and third stages of growth can
40°. The diffraction measurements can therefore not conﬁrm be made more quantitative by describing the clusters with a
the presence of facets with angles smaller than 40° as ob- modiﬁed unit cell. This cell is built up from unit blocks
served in the AFM studies. deﬁned by the in-plane 102 and b axis, and the c axis. In
this new description, several (h 0 l) facets can be formed,
with only small values of h and l. For example, the 14° facet
corresponds to a ¯01 facet with a terrace width of two unit
Film growth on SrTiO 3 001 initially proceeds in the 3D cells followed by a step of one unit cell height. The 100
island growth mode Volmer-Weber mode . The typical is- facet corresponds to the 55° faceting as measured with x-ray
land size is 50–200 nm with an island height of about 10 nm. diffraction. The angles of 7°, 14°, 18°, 22°, 30°, and 39° as
The islands are monocrystalline and show clear epitaxial be- observed in AFM measurements are identiﬁed as ¯04 , 1
havior: the fourfold symmetry of the substrate surface results ¯ ¯
102 , 101 , 403 , 101 , and 401 facets, respectively.
in four crystallographic blue-bronze orientations. Islands Note that this model predicts the clusters to be asymmetric
grow in the 201 direction with the b axis along the princi- when viewed along the b axis Fig. 5 a . The growth of
12 534 A. J. STEINFORT et al. 57
FIG. 5. A model for the cluster growth. The second stage of growth as described in the text is illustrated in the upper panel. Various facet
angles are schematically shown in a , which correspond to the angles determined from AFM data b . The third stage of growth is illustrated
in the lower panel. The growth of 201 slabs over the cluster facets is schematically shown in c . The overgrowth is conﬁrmed by STM
images of a cluster d showing different periodicities perpendicular to the b axis.
201 slabs over the faceted grains is schematically shown in V. CONCLUSIONS
Fig. 5 c . The angles between the ¯01 slabs and the surface
Highly textured ﬁlms are grown on SrTiO 3 001 sub-
are consistent with the x-ray diffraction data Fig. 3 b . strates. At the initial growth, heteroepitaxial monocrystalline
The overgrowth of the slabs is also conﬁrmed by STM islands form with a weak substrate-ﬁlm bonding. The blue
measurements.10 In Fig. 5 d an STM image of a cluster is bronze is fully relaxed, and orients with the in-plane b axis
shown. In this image periodic line structures are observed. In to the principal axes of the substrate. An orientation distri-
these lines the b-axis periodicity is present with a period of bution of 1.1° around these directions is observed. On thick
0.75 nm. The lines are the end points of tilted 201 slabs as ﬁlms, grains are considerably larger and the orientation
illustrated in Fig. 5 c . The periodicity perpendicular to the b spread increases. The major part of the grains remains ori-
axis is therefore determined by the facet angle over which ented with the b axis along the principal axes of the sub-
overgrowth occurs. The horizontal distance between 201 ¯ strate. A minor part of grains have additional orientations of
slabs is equal to d (2 01) /sin(tilt angle) with d (2 01) 0.83 nm.
¯ ¯ 27° and 45° with respect to the SrTiO 3 100 . In the out-of-
In Fig. 5 d we observe periodicities of 2.45 and 1.43 nm plane direction, the thick ﬁlms show additional orientations.
between the lines. These distances correspond to tilt angles The b axis remains oriented in-plane, but besides the
surface-parallel 201 slabs, a tilt of the slabs is observed. A
of 22° and 39°. We have made many STM images of blue-
bronze clusters. Most of the clusters contain a periodicity in correlation between the faceting of the clusters and the pre-
a direction perpendicular to the b axis. In all cases, we could ferred out-of-plane orientations is found. The data are fully
explained with a model including growth of 201 slabs over
identify a low-index facet angle that corresponds to the ob-
served period. facets of the clusters. The model indicates that the correlation
The overgrowth results in a correlation length that is length perpendicular to the b axis is smaller than the dimen-
smaller than the cluster size. This conclusion is consistent sions of the grains. This observation is consistent with elec-
with our electrical transport measurements on blue-bronze trical transport data, which show that the energy gap mea-
ﬁlms. In general, we ﬁnd an energy gap that is lower than the sured in ﬁlms grown on SrTiO 3 001 substrates is largely
observed values 520 K in bulk blue bronze. Films grown independent on the apparent grain size as deduced from SEM
on Al2 O3 012 show a systematic decrease of the energy gap pictures.
with decreasing grain size. Films grown at high temperatures
with large grains have an energy gap close to the bulk value.
For ﬁlms with submicron grains, the gap is reduced by 30%. The authors would like to thank P. W. F. Rutten and
Such a dependence is absent for ﬁlms grown on C. A. W. Bal for their careful AFM work, and K. R. Koops
SrTiO 3 (001): no matter how large the grain size, the appar- for the support by the STM measurements. We also want
ent gap deduced from electric transport measurements is al- to thank M. Nielsen and J. Baker for the assistance on
most constant around 400 K . Extrapolation of the results the diffraction experiments at the DESY synchrotron
obtained on the Al 2 O 3 012 substrates then yields that the in Hamburg. This work has been supported by The Nether-
grains seen by SEM on SrTiO 3 (001) must consist of smaller lands Foundation for Fundamental Research on Matter
clusters. FOM .
57 EPITAXIAL FILM GROWTH OF THE CHARGE- . . . 12 535
G. Gruner, Density Waves in Solids Addison-Wesley, Reading Low-Dimensional Electronic Properties of Molybdenum
MA, 1994 . Bronzes and Oxides, edited by C. Schlenker Kluwer, New
P. Monceau, in Electronic Properties of Inorganic Quasi-One York, 1989 , pp. 159–257.
Dimensional Compounds, edited by P. Monceau Reidel, Dor- 7
W. J. Schutte and J. L. de Boer, Acta Crystallogr., Sect. B: Struct.
drecht, 1985 , Vol. 2. Crystallogr. Cryst. Chem. 49, 579 1993 .
R. Peierls, Quantum Theory of Solids Oxford University Press, 8
A. J. Steinfort, Ph.D. thesis, Delft, The Netherlands, 1998 .
Oxford, 1955 , p. 108. 9
A. J. Steinfort, P. M. L. O. Scholte, A. Ettema, F. Tuinstra, M.
H. S. J. van der Zant, O. C. Mantel, C. Dekker, J. E. Mooij, and Nielsen, E. Landemark, D.-M. Smilgies, R. Feidenhans’l, G.
C. Træholt, Appl. Phys. Lett. 68, 3823 1996 . Falkenberg, L. Seehofer, and R. L. Johnson, Phys. Rev. Lett. 77,
O. C. Mantel, H. S. J. van der Zant, A. J. Steinfort, C. Dekker, C. 2009 1996 .
Træholt, and H. W. Zandbergen, Phys. Rev. B 55, 4817 1997 . 10
6 A. J. Steinfort and H. S. J. van der Zant unpublished .
C. Schlenker, J. Dumas, C. Escribe-Filippini, and H. Guyot, in